#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/08/4330809.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4330809
loop_
_publ_author_name
'Nikolay S. Abramchuk'
'Wilder Carrillo-Cabrera'
'Igor Veremchuk'
'Niels Oeschler'
'Andrei V. Olenev'
'Yurii Prots'
'Ulrich Burkhardt'
'Evgeny V. Dikarev'
'Yuri Grin'
'Andrei V. Shevelkov'
_publ_contact_author_address
;
Max-Planck-Institut für Chemische Physik fester Stoffe
Nöthnitzer Str. 40
01187 Dresden
Germany
;
_publ_contact_author_email       Nikolay.Abramchuk@cpfs.mpg.de
_publ_contact_author_fax         49(351)46464002
_publ_contact_author_name        'Abramchuk, Nikolay'
_publ_contact_author_phone       49(351)46462236
_publ_section_title
;
 Homo- and Heterovalent Substitutions in the New Clathrates I
 Si30P16Te8-xSex and Si30+xP16-xTe8-xBrx: Synthesis, Crystal Structure,
 and Thermoelectric Properties
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              11396
_journal_page_last               11405
_journal_paper_doi               10.1021/ic3010097
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'Br1.52 P13.54 Si32.46 Te6.01'
_chemical_formula_weight         2219.47
_space_group_IT_number           200
_space_group_name_Hall           '-P 2 2 3'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 2 2 3'
_symmetry_space_group_name_H-M   'P m -3'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   9.9863(4)
_cell_length_b                   9.9863(4)
_cell_length_c                   9.9863(4)
_cell_measurement_temperature    298
_cell_volume                     995.90(7)
_computing_cell_refinement       WinGX
_computing_data_collection       'CrystalClear (Rigaku Inc., 2008)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2008)'
_computing_structure_refinement  WinGX
_diffrn_ambient_temperature      298
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Rigaku AFC7'
_diffrn_measurement_method       dtprofit.ref
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0456
_diffrn_reflns_av_sigmaI/netI    0.0236
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            5828
_diffrn_reflns_theta_full        29.96
_diffrn_reflns_theta_max         29.96
_diffrn_reflns_theta_min         2.04
_exptl_absorpt_coefficient_mu    7.415
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.7137
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            'gray metallic'
_exptl_crystal_density_diffrn    3.701
_exptl_crystal_description       cube
_exptl_crystal_F_000             1023
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_refine_ls_extinction_coef       0.0036(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.461
_refine_ls_matrix_type           full
_refine_ls_number_parameters     34
_refine_ls_number_reflns         571
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.461
_refine_ls_R_factor_all          0.0309
_refine_ls_R_factor_gt           0.0306
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0375P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0833
_refine_ls_wR_factor_ref         0.0834
_reflns_number_gt                567
_reflns_number_total             571
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic3010097_si_002_12.cif
_cod_data_source_block           '[Si,P]46Te6.01Br1.52_crystal_V'
_cod_original_cell_volume        995.90(2)
_cod_original_formula_sum        'P13.54 Br1.52 Si32.46 Te6.01'
_cod_database_code               4330809
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x, -y, -z'
'-x, y, -z'
'y, z, x'
'-y, -z, x'
'y, -z, -x'
'-y, z, -x'
'z, x, y'
'-z, x, -y'
'-z, -x, y'
'z, -x, -y'
'-x, -y, -z'
'x, y, -z'
'-x, y, z'
'x, -y, z'
'-y, -z, -x'
'y, z, -x'
'-y, z, x'
'y, -z, x'
'-z, -x, -y'
'z, -x, y'
'z, x, -y'
'-z, x, y'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Te1 Te 0.26055(8) 0.0000 0.5000 0.0195(2) Uani 0.915(17) 4 d SP
Br3 Br 0.26055(8) 0.0000 0.5000 0.0195(2) Uani 0.085(17) 4 d SP
Br1 Br 0.5000 0.5000 0.5000 0.0089(11) Uani 0.494(9) 24 d SP
Br2A Br 0.0000 0.0000 0.0000 0.0118(4) Uani 0.45(2) 24 d SP
Te2B Te 0.0000 0.0000 0.0000 0.0118(4) Uani 0.55(2) 24 d SP
Si1 Si 0.18457(12) 0.18457(12) 0.18457(12) 0.0103(5) Uani 1 3 d S
P2 P 0.31676(11) 0.31676(11) 0.31676(11) 0.0105(4) Uani 1 3 d S
P3 P 0.0000 0.11740(17) 0.30895(18) 0.0146(4) Uani 1 2 d S
Si4 Si 0.19067(17) 0.38313(17) 0.5000 0.0123(4) Uani 1 2 d S
Si5 Si 0.0000 0.2478(3) 0.5000 0.0097(5) Uani 1 4 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Si4 Te1 Si4 41.79(6) 10_656 9
Si4 Te1 Si4 71.18(5) 10_656 21_656
Si4 Te1 Si4 86.09(5) 9 21_656
Si4 Te1 Si4 86.09(5) 10_656 22
Si4 Te1 Si4 71.18(5) 9 22
Si4 Te1 Si4 41.79(6) 21_656 22
Si4 Te1 P3 161.97(4) 10_656 2
Si4 Te1 P3 123.67(4) 9 2
Si4 Te1 P3 123.60(4) 21_656 2
Si4 Te1 P3 99.03(3) 22 2
Si4 Te1 P3 123.67(4) 10_656 13_556
Si4 Te1 P3 161.97(4) 9 13_556
Si4 Te1 P3 99.03(3) 21_656 13_556
Si4 Te1 P3 123.60(4) 22 13_556
P3 Te1 P3 67.53(5) 2 13_556
Si4 Te1 P3 123.60(4) 10_656 .
Si4 Te1 P3 99.03(3) 9 .
Si4 Te1 P3 161.97(4) 21_656 .
Si4 Te1 P3 123.67(4) 22 .
P3 Te1 P3 39.94(6) 2 .
P3 Te1 P3 81.43(5) 13_556 .
Si4 Te1 P3 99.03(3) 10_656 14_556
Si4 Te1 P3 123.60(4) 9 14_556
Si4 Te1 P3 123.67(4) 21_656 14_556
Si4 Te1 P3 161.97(4) 22 14_556
P3 Te1 P3 81.43(5) 2 14_556
P3 Te1 P3 39.94(6) 13_556 14_556
P3 Te1 P3 67.53(5) . 14_556
Si4 Te1 Si5 40.37(3) 10_656 21_656
Si4 Te1 Si5 75.85(4) 9 21_656
Si4 Te1 Si5 40.37(3) 21_656 21_656
Si4 Te1 Si5 75.85(4) 22 21_656
P3 Te1 Si5 157.66(3) 2 21_656
P3 Te1 Si5 96.82(4) 13_556 21_656
P3 Te1 Si5 157.66(3) . 21_656
P3 Te1 Si5 96.82(4) 14_556 21_656
Si4 Te1 Si5 75.85(4) 10_656 9
Si4 Te1 Si5 40.37(3) 9 9
Si4 Te1 Si5 75.85(4) 21_656 9
Si4 Te1 Si5 40.37(3) 22 9
P3 Te1 Si5 96.82(4) 2 9
P3 Te1 Si5 157.66(3) 13_556 9
P3 Te1 Si5 96.82(4) . 9
P3 Te1 Si5 157.66(3) 14_556 9
Si5 Te1 Si5 92.97(7) 21_656 9
Si4 Te1 Si5 158.53(3) 10_656 13_556
Si4 Te1 Si5 158.53(3) 9 13_556
Si4 Te1 Si5 97.38(4) 21_656 13_556
Si4 Te1 Si5 97.38(4) 22 13_556
P3 Te1 Si5 38.32(3) 2 13_556
P3 Te1 Si5 38.32(3) 13_556 13_556
P3 Te1 Si5 71.71(4) . 13_556
P3 Te1 Si5 71.71(4) 14_556 13_556
Si5 Te1 Si5 119.929(2) 21_656 13_556
Si5 Te1 Si5 119.929(2) 9 13_556
Si4 Te1 Si5 97.38(4) 10_656 .
Si4 Te1 Si5 97.38(4) 9 .
Si4 Te1 Si5 158.53(3) 21_656 .
Si4 Te1 Si5 158.53(3) 22 .
P3 Te1 Si5 71.71(4) 2 .
P3 Te1 Si5 71.71(4) 13_556 .
P3 Te1 Si5 38.32(3) . .
P3 Te1 Si5 38.32(3) 14_556 .
Si5 Te1 Si5 119.929(2) 21_656 .
Si5 Te1 Si5 119.929(2) 9 .
Si5 Te1 Si5 87.13(7) 13_556 .
Si4 Te1 P2 38.24(3) 10_656 14_556
Si4 Te1 P2 64.39(4) 9 14_556
Si4 Te1 P2 102.15(3) 21_656 14_556
Si4 Te1 P2 124.30(3) 22 14_556
P3 Te1 P2 133.03(3) 2 14_556
P3 Te1 P2 97.60(4) 13_556 14_556
P3 Te1 P2 95.62(3) . 14_556
P3 Te1 P2 63.11(3) 14_556 14_556
Si5 Te1 P2 62.389(9) 21_656 14_556
Si5 Te1 P2 104.74(4) 9 14_556
Si5 Te1 P2 134.40(4) 13_556 14_556
Si5 Te1 P2 61.34(3) . 14_556
Si4 Te1 P2 124.30(3) 10_656 16
Si4 Te1 P2 102.15(3) 9 16
Si4 Te1 P2 64.39(4) 21_656 16
Si4 Te1 P2 38.24(3) 22 16
P3 Te1 P2 63.11(3) 2 16
P3 Te1 P2 95.62(3) 13_556 16
P3 Te1 P2 97.60(4) . 16
P3 Te1 P2 133.03(3) 14_556 16
Si5 Te1 P2 104.74(4) 21_656 16
Si5 Te1 P2 62.389(9) 9 16
Si5 Te1 P2 61.34(2) 13_556 16
Si5 Te1 P2 134.40(4) . 16
P2 Te1 P2 162.54(4) 14_556 16
Si4 Te1 P2 64.39(4) 10_656 .
Si4 Te1 P2 38.24(3) 9 .
Si4 Te1 P2 124.30(3) 21_656 .
Si4 Te1 P2 102.15(3) 22 .
P3 Te1 P2 97.60(4) 2 .
P3 Te1 P2 133.03(3) 13_556 .
P3 Te1 P2 63.11(3) . .
P3 Te1 P2 95.62(3) 14_556 .
Si5 Te1 P2 104.74(4) 21_656 .
Si5 Te1 P2 62.389(9) 9 .
Si5 Te1 P2 134.40(4) 13_556 .
Si5 Te1 P2 61.34(2) . .
P2 Te1 P2 59.33(5) 14_556 .
P2 Te1 P2 117.64(4) 16 .
Si4 Te1 P2 102.15(3) 10_656 3_556
Si4 Te1 P2 124.30(3) 9 3_556
Si4 Te1 P2 38.24(3) 21_656 3_556
Si4 Te1 P2 64.39(4) 22 3_556
P3 Te1 P2 95.62(3) 2 3_556
P3 Te1 P2 63.11(3) 13_556 3_556
P3 Te1 P2 133.03(3) . 3_556
P3 Te1 P2 97.60(4) 14_556 3_556
Si5 Te1 P2 62.389(9) 21_656 3_556
Si5 Te1 P2 104.74(4) 9 3_556
Si5 Te1 P2 61.34(2) 13_556 3_556
Si5 Te1 P2 134.40(4) . 3_556
P2 Te1 P2 117.64(4) 14_556 3_556
P2 Te1 P2 59.33(5) 16 3_556
P2 Te1 P2 162.54(4) . 3_556
Si4 Te1 Si1 137.55(3) 10_656 16
Si4 Te1 Si1 97.76(3) 9 16
Si4 Te1 Si1 99.35(4) 21_656 16
Si4 Te1 Si1 63.87(4) 22 16
P3 Te1 Si1 37.55(3) 2 16
P3 Te1 Si1 98.42(3) 13_556 16
P3 Te1 Si1 62.93(4) . 16
P3 Te1 Si1 118.96(3) 14_556 16
Si5 Te1 Si1 138.85(4) 21_656 16
Si5 Te1 Si1 61.79(2) 9 16
Si5 Te1 Si1 60.774(9) 13_556 16
Si5 Te1 Si1 101.14(4) . 16
P2 Te1 Si1 150.71(3) 14_556 16
P2 Te1 Si1 35.87(4) 16 16
P2 Te1 Si1 92.05(4) . 16
P2 Te1 Si1 91.50(4) 3_556 16
Si4 Te1 Si1 63.87(4) 10_656 14_556
Si4 Te1 Si1 99.35(4) 9 14_556
Si4 Te1 Si1 97.76(3) 21_656 14_556
Si4 Te1 Si1 137.55(3) 22 14_556
P3 Te1 Si1 118.96(3) 2 14_556
P3 Te1 Si1 62.93(4) 13_556 14_556
P3 Te1 Si1 98.42(3) . 14_556
P3 Te1 Si1 37.55(3) 14_556 14_556
Si5 Te1 Si1 61.79(2) 21_656 14_556
Si5 Te1 Si1 138.85(4) 9 14_556
Si5 Te1 Si1 101.14(4) 13_556 14_556
Si5 Te1 Si1 60.774(9) . 14_556
P2 Te1 Si1 35.87(4) 14_556 14_556
P2 Te1 Si1 150.71(3) 16 14_556
P2 Te1 Si1 91.50(4) . 14_556
P2 Te1 Si1 92.05(4) 3_556 14_556
Si1 Te1 Si1 156.51(4) 16 14_556
Si4 Te1 Si1 99.35(4) 10_656 .
Si4 Te1 Si1 63.87(4) 9 .
Si4 Te1 Si1 137.55(3) 21_656 .
Si4 Te1 Si1 97.76(3) 22 .
P3 Te1 Si1 62.93(4) 2 .
P3 Te1 Si1 118.96(3) 13_556 .
P3 Te1 Si1 37.55(3) . .
P3 Te1 Si1 98.42(3) 14_556 .
Si5 Te1 Si1 138.85(4) 21_656 .
Si5 Te1 Si1 61.79(2) 9 .
Si5 Te1 Si1 101.14(4) 13_556 .
Si5 Te1 Si1 60.774(9) . .
P2 Te1 Si1 91.50(4) 14_556 .
P2 Te1 Si1 92.05(4) 16 .
P2 Te1 Si1 35.87(4) . .
P2 Te1 Si1 150.71(3) 3_556 .
Si1 Te1 Si1 59.27(5) 16 .
Si1 Te1 Si1 115.35(4) 14_556 .
Si4 Te1 Si1 97.76(3) 10_656 3_556
Si4 Te1 Si1 137.55(3) 9 3_556
Si4 Te1 Si1 63.87(4) 21_656 3_556
Si4 Te1 Si1 99.35(4) 22 3_556
P3 Te1 Si1 98.42(3) 2 3_556
P3 Te1 Si1 37.55(3) 13_556 3_556
P3 Te1 Si1 118.96(3) . 3_556
P3 Te1 Si1 62.93(4) 14_556 3_556
Si5 Te1 Si1 61.79(2) 21_656 3_556
Si5 Te1 Si1 138.85(4) 9 3_556
Si5 Te1 Si1 60.774(9) 13_556 3_556
Si5 Te1 Si1 101.14(4) . 3_556
P2 Te1 Si1 92.05(4) 14_556 3_556
P2 Te1 Si1 91.50(4) 16 3_556
P2 Te1 Si1 150.71(3) . 3_556
P2 Te1 Si1 35.87(4) 3_556 3_556
Si1 Te1 Si1 115.35(4) 16 3_556
Si1 Te1 Si1 59.27(5) 14_556 3_556
Si1 Te1 Si1 156.51(4) . 3_556
Si4 Te1 P3 105.20(4) 10_656 9
Si4 Te1 P3 63.54(4) 9 9
Si4 Te1 P3 105.20(4) 21_656 9
Si4 Te1 P3 63.54(4) 22 9
P3 Te1 P3 62.86(5) 2 9
P3 Te1 P3 130.278(17) 13_556 9
P3 Te1 P3 62.86(5) . 9
P3 Te1 P3 130.278(17) 14_556 9
Si5 Te1 P3 129.28(5) 21_656 9
Si5 Te1 P3 36.30(4) 9 9
Si5 Te1 P3 95.22(2) 13_556 9
Si5 Te1 P3 95.22(2) . 9
P2 Te1 P3 118.16(3) 14_556 9
P2 Te1 P3 59.33(2) 16 9
P2 Te1 P3 59.33(2) . 9
P2 Te1 P3 118.16(3) 3_556 9
Si1 Te1 P3 35.63(2) 16 9
Si1 Te1 P3 149.76(2) 14_556 9
Si1 Te1 P3 35.63(2) . 9
Si1 Te1 P3 149.76(2) 3_556 9
Si4 Te1 P3 63.54(4) 10_656 23_556
Si4 Te1 P3 105.20(4) 9 23_556
Si4 Te1 P3 63.54(4) 21_656 23_556
Si4 Te1 P3 105.20(4) 22 23_556
P3 Te1 P3 130.278(17) 2 23_556
P3 Te1 P3 62.86(5) 13_556 23_556
P3 Te1 P3 130.278(17) . 23_556
P3 Te1 P3 62.86(5) 14_556 23_556
Si5 Te1 P3 36.30(4) 21_656 23_556
Si5 Te1 P3 129.28(5) 9 23_556
Si5 Te1 P3 95.22(2) 13_556 23_556
Si5 Te1 P3 95.22(2) . 23_556
P2 Te1 P3 59.33(2) 14_556 23_556
P2 Te1 P3 118.16(3) 16 23_556
P2 Te1 P3 118.16(3) . 23_556
P2 Te1 P3 59.33(2) 3_556 23_556
Si1 Te1 P3 149.76(2) 16 23_556
Si1 Te1 P3 35.63(2) 14_556 23_556
Si1 Te1 P3 149.76(2) . 23_556
Si1 Te1 P3 35.63(2) 3_556 23_556
P3 Te1 P3 165.58(6) 9 23_556
Si4 Te1 Si4 134.720(18) 10_656 3_556
Si4 Te1 Si4 134.720(18) 9 3_556
Si4 Te1 Si4 63.81(5) 21_656 3_556
Si4 Te1 Si4 63.81(5) 22 3_556
P3 Te1 Si4 61.84(3) 2 3_556
P3 Te1 Si4 61.84(3) 13_556 3_556
P3 Te1 Si4 101.54(4) . 3_556
P3 Te1 Si4 101.54(4) 14_556 3_556
Si5 Te1 Si4 97.097(19) 21_656 3_556
Si5 Te1 Si4 97.097(19) 9 3_556
Si5 Te1 Si4 36.10(4) 13_556 3_556
Si5 Te1 Si4 123.23(5) . 3_556
P2 Te1 Si4 150.33(3) 14_556 3_556
P2 Te1 Si4 35.468(17) 16 3_556
P2 Te1 Si4 150.33(3) . 3_556
P2 Te1 Si4 35.468(17) 3_556 3_556
Si1 Te1 Si4 58.47(2) 16 3_556
Si1 Te1 Si4 116.74(3) 14_556 3_556
Si1 Te1 Si4 116.74(3) . 3_556
Si1 Te1 Si4 58.47(2) 3_556 3_556
P3 Te1 Si4 91.290(5) 9 3_556
P3 Te1 Si4 91.290(5) 23_556 3_556
Si4 Te1 Si4 63.81(5) 10_656 .
Si4 Te1 Si4 63.81(5) 9 .
Si4 Te1 Si4 134.720(18) 21_656 .
Si4 Te1 Si4 134.720(18) 22 .
P3 Te1 Si4 101.54(4) 2 .
P3 Te1 Si4 101.54(4) 13_556 .
P3 Te1 Si4 61.84(3) . .
P3 Te1 Si4 61.84(3) 14_556 .
Si5 Te1 Si4 97.097(19) 21_656 .
Si5 Te1 Si4 97.097(19) 9 .
Si5 Te1 Si4 123.23(5) 13_556 .
Si5 Te1 Si4 36.10(4) . .
P2 Te1 Si4 35.468(17) 14_556 .
P2 Te1 Si4 150.33(3) 16 .
P2 Te1 Si4 35.468(17) . .
P2 Te1 Si4 150.33(3) 3_556 .
Si1 Te1 Si4 116.74(3) 16 .
Si1 Te1 Si4 58.47(2) 14_556 .
Si1 Te1 Si4 58.47(2) . .
Si1 Te1 Si4 116.74(3) 3_556 .
P3 Te1 Si4 91.290(5) 9 .
P3 Te1 Si4 91.290(5) 23_556 .
Si4 Te1 Si4 159.33(6) 3_556 .
Si4 Te1 Te1 43.04(2) 10_656 13_656
Si4 Te1 Te1 43.04(2) 9 13_656
Si4 Te1 Te1 43.04(2) 21_656 13_656
Si4 Te1 Te1 43.04(2) 22 13_656
P3 Te1 Te1 139.28(2) 2 13_656
P3 Te1 Te1 139.28(2) 13_556 13_656
P3 Te1 Te1 139.28(2) . 13_656
P3 Te1 Te1 139.28(2) 14_556 13_656
Si5 Te1 Te1 46.49(3) 21_656 13_656
Si5 Te1 Te1 46.49(3) 9 13_656
Si5 Te1 Te1 136.44(3) 13_556 13_656
Si5 Te1 Te1 136.44(3) . 13_656
P2 Te1 Te1 81.27(2) 14_556 13_656
P2 Te1 Te1 81.27(2) 16 13_656
P2 Te1 Te1 81.27(2) . 13_656
P2 Te1 Te1 81.27(2) 3_556 13_656
Si1 Te1 Te1 101.75(2) 16 13_656
Si1 Te1 Te1 101.75(2) 14_556 13_656
Si1 Te1 Te1 101.75(2) . 13_656
Si1 Te1 Te1 101.75(2) 3_556 13_656
P3 Te1 Te1 82.79(3) 9 13_656
P3 Te1 Te1 82.79(3) 23_556 13_656
Si4 Te1 Te1 100.34(3) 3_556 13_656
Si4 Te1 Te1 100.34(3) . 13_656
P2 Br1 P2 180.00(3) 13_666 .
P2 Br1 P2 109.5 13_666 16_565
P2 Br1 P2 70.5 . 16_565
P2 Br1 P2 70.5 13_666 4_656
P2 Br1 P2 109.5 . 4_656
P2 Br1 P2 180.0 16_565 4_656
P2 Br1 P2 109.5 13_666 15_655
P2 Br1 P2 70.5 . 15_655
P2 Br1 P2 109.5 16_565 15_655
P2 Br1 P2 70.5 4_656 15_655
P2 Br1 P2 70.5 13_666 3_566
P2 Br1 P2 109.5 . 3_566
P2 Br1 P2 70.5 16_565 3_566
P2 Br1 P2 109.5 4_656 3_566
P2 Br1 P2 180.0 15_655 3_566
P2 Br1 P2 109.5 13_666 14_556
P2 Br1 P2 70.5 . 14_556
P2 Br1 P2 109.5 16_565 14_556
P2 Br1 P2 70.5 4_656 14_556
P2 Br1 P2 109.5 15_655 14_556
P2 Br1 P2 70.5 3_566 14_556
P2 Br1 P2 70.5 13_666 2_665
P2 Br1 P2 109.5 . 2_665
P2 Br1 P2 70.5 16_565 2_665
P2 Br1 P2 109.5 4_656 2_665
P2 Br1 P2 70.5 15_655 2_665
P2 Br1 P2 109.5 3_566 2_665
P2 Br1 P2 180.00(3) 14_556 2_665
P2 Br1 Si4 41.915(15) 13_666 21_666
P2 Br1 Si4 138.085(15) . 21_666
P2 Br1 Si4 70.36(2) 16_565 21_666
P2 Br1 Si4 109.64(2) 4_656 21_666
P2 Br1 Si4 138.085(15) 15_655 21_666
P2 Br1 Si4 41.915(15) 3_566 21_666
P2 Br1 Si4 109.64(2) 14_556 21_666
P2 Br1 Si4 70.36(2) 2_665 21_666
P2 Br1 Si4 41.915(15) 13_666 17_666
P2 Br1 Si4 138.085(15) . 17_666
P2 Br1 Si4 138.085(15) 16_565 17_666
P2 Br1 Si4 41.915(15) 4_656 17_666
P2 Br1 Si4 109.64(2) 15_655 17_666
P2 Br1 Si4 70.36(2) 3_566 17_666
P2 Br1 Si4 70.36(2) 14_556 17_666
P2 Br1 Si4 109.64(2) 2_665 17_666
Si4 Br1 Si4 70.69(2) 21_666 17_666
P2 Br1 Si4 41.915(15) 13_666 13_666
P2 Br1 Si4 138.085(15) . 13_666
P2 Br1 Si4 109.64(2) 16_565 13_666
P2 Br1 Si4 70.36(2) 4_656 13_666
P2 Br1 Si4 70.36(2) 15_655 13_666
P2 Br1 Si4 109.64(2) 3_566 13_666
P2 Br1 Si4 138.085(15) 14_556 13_666
P2 Br1 Si4 41.915(15) 2_665 13_666
Si4 Br1 Si4 70.69(2) 21_666 13_666
Si4 Br1 Si4 70.69(2) 17_666 13_666
P2 Br1 Si4 138.085(15) 13_666 9
P2 Br1 Si4 41.915(15) . 9
P2 Br1 Si4 109.64(2) 16_565 9
P2 Br1 Si4 70.36(2) 4_656 9
P2 Br1 Si4 41.915(15) 15_655 9
P2 Br1 Si4 138.085(15) 3_566 9
P2 Br1 Si4 70.36(2) 14_556 9
P2 Br1 Si4 109.64(2) 2_665 9
Si4 Br1 Si4 180.0 21_666 9
Si4 Br1 Si4 109.31(2) 17_666 9
Si4 Br1 Si4 109.31(2) 13_666 9
P2 Br1 Si4 138.085(15) 13_666 .
P2 Br1 Si4 41.915(15) . .
P2 Br1 Si4 70.36(2) 16_565 .
P2 Br1 Si4 109.64(2) 4_656 .
P2 Br1 Si4 109.64(2) 15_655 .
P2 Br1 Si4 70.36(2) 3_566 .
P2 Br1 Si4 41.915(15) 14_556 .
P2 Br1 Si4 138.085(15) 2_665 .
Si4 Br1 Si4 109.31(2) 21_666 .
Si4 Br1 Si4 109.31(2) 17_666 .
Si4 Br1 Si4 180.00(5) 13_666 .
Si4 Br1 Si4 70.69(2) 9 .
P2 Br1 Si4 138.085(15) 13_666 5
P2 Br1 Si4 41.915(15) . 5
P2 Br1 Si4 41.915(15) 16_565 5
P2 Br1 Si4 138.085(15) 4_656 5
P2 Br1 Si4 70.36(2) 15_655 5
P2 Br1 Si4 109.64(2) 3_566 5
P2 Br1 Si4 109.64(2) 14_556 5
P2 Br1 Si4 70.36(2) 2_665 5
Si4 Br1 Si4 109.31(2) 21_666 5
Si4 Br1 Si4 180.0 17_666 5
Si4 Br1 Si4 109.31(2) 13_666 5
Si4 Br1 Si4 70.69(2) 9 5
Si4 Br1 Si4 70.69(2) . 5
P2 Br1 Si4 109.64(2) 13_666 10_656
P2 Br1 Si4 70.36(2) . 10_656
P2 Br1 Si4 138.085(15) 16_565 10_656
P2 Br1 Si4 41.915(15) 4_656 10_656
P2 Br1 Si4 70.36(2) 15_655 10_656
P2 Br1 Si4 109.64(2) 3_566 10_656
P2 Br1 Si4 41.915(15) 14_556 10_656
P2 Br1 Si4 138.085(15) 2_665 10_656
Si4 Br1 Si4 138.61(6) 21_666 10_656
Si4 Br1 Si4 70.69(2) 17_666 10_656
Si4 Br1 Si4 109.31(2) 13_666 10_656
Si4 Br1 Si4 41.39(6) 9 10_656
Si4 Br1 Si4 70.69(2) . 10_656
Si4 Br1 Si4 109.31(2) 5 10_656
P2 Br1 Si4 109.64(2) 13_666 6_665
P2 Br1 Si4 70.36(2) . 6_665
P2 Br1 Si4 70.36(2) 16_565 6_665
P2 Br1 Si4 109.64(2) 4_656 6_665
P2 Br1 Si4 41.915(15) 15_655 6_665
P2 Br1 Si4 138.085(15) 3_566 6_665
P2 Br1 Si4 138.085(15) 14_556 6_665
P2 Br1 Si4 41.915(15) 2_665 6_665
Si4 Br1 Si4 109.31(2) 21_666 6_665
Si4 Br1 Si4 138.61(6) 17_666 6_665
Si4 Br1 Si4 70.69(2) 13_666 6_665
Si4 Br1 Si4 70.69(2) 9 6_665
Si4 Br1 Si4 109.31(2) . 6_665
Si4 Br1 Si4 41.39(6) 5 6_665
Si4 Br1 Si4 109.31(2) 10_656 6_665
P2 Br1 Si4 109.64(2) 13_666 3_566
P2 Br1 Si4 70.36(2) . 3_566
P2 Br1 Si4 41.915(15) 16_565 3_566
P2 Br1 Si4 138.085(15) 4_656 3_566
P2 Br1 Si4 138.085(15) 15_655 3_566
P2 Br1 Si4 41.915(15) 3_566 3_566
P2 Br1 Si4 70.36(2) 14_556 3_566
P2 Br1 Si4 109.64(2) 2_665 3_566
Si4 Br1 Si4 70.69(2) 21_666 3_566
Si4 Br1 Si4 109.31(2) 17_666 3_566
Si4 Br1 Si4 138.61(6) 13_666 3_566
Si4 Br1 Si4 109.31(2) 9 3_566
Si4 Br1 Si4 41.39(6) . 3_566
Si4 Br1 Si4 70.69(2) 5 3_566
Si4 Br1 Si4 109.31(2) 10_656 3_566
Si4 Br1 Si4 109.31(2) 6_665 3_566
P2 Br1 Si4 70.36(2) 13_666 22_565
P2 Br1 Si4 109.64(2) . 22_565
P2 Br1 Si4 41.915(15) 16_565 22_565
P2 Br1 Si4 138.085(15) 4_656 22_565
P2 Br1 Si4 109.64(2) 15_655 22_565
P2 Br1 Si4 70.36(2) 3_566 22_565
P2 Br1 Si4 138.085(15) 14_556 22_565
P2 Br1 Si4 41.915(15) 2_665 22_565
Si4 Br1 Si4 41.39(6) 21_666 22_565
Si4 Br1 Si4 109.31(2) 17_666 22_565
Si4 Br1 Si4 70.69(2) 13_666 22_565
Si4 Br1 Si4 138.61(6) 9 22_565
Si4 Br1 Si4 109.31(2) . 22_565
Si4 Br1 Si4 70.69(2) 5 22_565
Si4 Br1 Si4 180.0 10_656 22_565
Si4 Br1 Si4 70.69(2) 6_665 22_565
Si4 Br1 Si4 70.69(2) 3_566 22_565
P2 Br1 Si4 70.36(2) 13_666 18_556
P2 Br1 Si4 109.64(2) . 18_556
P2 Br1 Si4 109.64(2) 16_565 18_556
P2 Br1 Si4 70.36(2) 4_656 18_556
P2 Br1 Si4 138.085(15) 15_655 18_556
P2 Br1 Si4 41.915(15) 3_566 18_556
P2 Br1 Si4 41.915(15) 14_556 18_556
P2 Br1 Si4 138.085(15) 2_665 18_556
Si4 Br1 Si4 70.69(2) 21_666 18_556
Si4 Br1 Si4 41.39(6) 17_666 18_556
Si4 Br1 Si4 109.31(2) 13_666 18_556
Si4 Br1 Si4 109.31(2) 9 18_556
Si4 Br1 Si4 70.69(2) . 18_556
Si4 Br1 Si4 138.61(6) 5 18_556
Si4 Br1 Si4 70.69(2) 10_656 18_556
Si4 Br1 Si4 180.0 6_665 18_556
Si4 Br1 Si4 70.69(2) 3_566 18_556
Si4 Br1 Si4 109.31(2) 22_565 18_556
P2 Br1 Si4 70.36(2) 13_666 15_655
P2 Br1 Si4 109.64(2) . 15_655
P2 Br1 Si4 138.085(15) 16_565 15_655
P2 Br1 Si4 41.915(15) 4_656 15_655
P2 Br1 Si4 41.915(15) 15_655 15_655
P2 Br1 Si4 138.085(15) 3_566 15_655
P2 Br1 Si4 109.64(2) 14_556 15_655
P2 Br1 Si4 70.36(2) 2_665 15_655
Si4 Br1 Si4 109.31(2) 21_666 15_655
Si4 Br1 Si4 70.69(2) 17_666 15_655
Si4 Br1 Si4 41.39(6) 13_666 15_655
Si4 Br1 Si4 70.69(2) 9 15_655
Si4 Br1 Si4 138.61(6) . 15_655
Si4 Br1 Si4 109.31(2) 5 15_655
Si4 Br1 Si4 70.69(2) 10_656 15_655
Si4 Br1 Si4 70.69(2) 6_665 15_655
Si4 Br1 Si4 180.0 3_566 15_655
Si4 Br1 Si4 109.31(2) 22_565 15_655
Si4 Br1 Si4 109.31(2) 18_556 15_655
P2 Br1 Si1 180.00(2) 13_666 .
P2 Br1 Si1 0.00(2) . .
P2 Br1 Si1 70.5 16_565 .
P2 Br1 Si1 109.5 4_656 .
P2 Br1 Si1 70.5 15_655 .
P2 Br1 Si1 109.5 3_566 .
P2 Br1 Si1 70.5 14_556 .
P2 Br1 Si1 109.5 2_665 .
Si4 Br1 Si1 138.085(15) 21_666 .
Si4 Br1 Si1 138.085(15) 17_666 .
Si4 Br1 Si1 138.085(15) 13_666 .
Si4 Br1 Si1 41.915(15) 9 .
Si4 Br1 Si1 41.915(15) . .
Si4 Br1 Si1 41.915(15) 5 .
Si4 Br1 Si1 70.36(2) 10_656 .
Si4 Br1 Si1 70.36(2) 6_665 .
Si4 Br1 Si1 70.36(2) 3_566 .
Si4 Br1 Si1 109.64(2) 22_565 .
Si4 Br1 Si1 109.64(2) 18_556 .
Si4 Br1 Si1 109.64(2) 15_655 .
P2 Br1 Si1 0.00(2) 13_666 13_666
P2 Br1 Si1 180.000(19) . 13_666
P2 Br1 Si1 109.5 16_565 13_666
P2 Br1 Si1 70.5 4_656 13_666
P2 Br1 Si1 109.5 15_655 13_666
P2 Br1 Si1 70.5 3_566 13_666
P2 Br1 Si1 109.5 14_556 13_666
P2 Br1 Si1 70.5 2_665 13_666
Si4 Br1 Si1 41.915(15) 21_666 13_666
Si4 Br1 Si1 41.915(15) 17_666 13_666
Si4 Br1 Si1 41.915(15) 13_666 13_666
Si4 Br1 Si1 138.085(15) 9 13_666
Si4 Br1 Si1 138.085(15) . 13_666
Si4 Br1 Si1 138.085(15) 5 13_666
Si4 Br1 Si1 109.64(2) 10_656 13_666
Si4 Br1 Si1 109.64(2) 6_665 13_666
Si4 Br1 Si1 109.64(2) 3_566 13_666
Si4 Br1 Si1 70.36(2) 22_565 13_666
Si4 Br1 Si1 70.36(2) 18_556 13_666
Si4 Br1 Si1 70.36(2) 15_655 13_666
Si1 Br1 Si1 180.0 . 13_666
P2 Br1 Si1 109.5 13_666 16_565
P2 Br1 Si1 70.5 . 16_565
P2 Br1 Si1 0.000(19) 16_565 16_565
P2 Br1 Si1 180.000(19) 4_656 16_565
P2 Br1 Si1 109.5 15_655 16_565
P2 Br1 Si1 70.5 3_566 16_565
P2 Br1 Si1 109.5 14_556 16_565
P2 Br1 Si1 70.5 2_665 16_565
Si4 Br1 Si1 70.36(2) 21_666 16_565
Si4 Br1 Si1 138.085(15) 17_666 16_565
Si4 Br1 Si1 109.64(2) 13_666 16_565
Si4 Br1 Si1 109.64(2) 9 16_565
Si4 Br1 Si1 70.36(2) . 16_565
Si4 Br1 Si1 41.915(15) 5 16_565
Si4 Br1 Si1 138.085(15) 10_656 16_565
Si4 Br1 Si1 70.36(2) 6_665 16_565
Si4 Br1 Si1 41.915(15) 3_566 16_565
Si4 Br1 Si1 41.915(15) 22_565 16_565
Si4 Br1 Si1 109.64(2) 18_556 16_565
Si4 Br1 Si1 138.085(15) 15_655 16_565
Si1 Br1 Si1 70.5 . 16_565
Si1 Br1 Si1 109.5 13_666 16_565
P2 Br1 Si1 70.5 13_666 4_656
P2 Br1 Si1 109.5 . 4_656
P2 Br1 Si1 180.000(19) 16_565 4_656
P2 Br1 Si1 0.000(19) 4_656 4_656
P2 Br1 Si1 70.5 15_655 4_656
P2 Br1 Si1 109.5 3_566 4_656
P2 Br1 Si1 70.5 14_556 4_656
P2 Br1 Si1 109.5 2_665 4_656
Si4 Br1 Si1 109.64(2) 21_666 4_656
Si4 Br1 Si1 41.915(15) 17_666 4_656
Si4 Br1 Si1 70.36(2) 13_666 4_656
Si4 Br1 Si1 70.36(2) 9 4_656
Si4 Br1 Si1 109.64(2) . 4_656
Si4 Br1 Si1 138.085(15) 5 4_656
Si4 Br1 Si1 41.915(15) 10_656 4_656
Si4 Br1 Si1 109.64(2) 6_665 4_656
Si4 Br1 Si1 138.085(15) 3_566 4_656
Si4 Br1 Si1 138.085(15) 22_565 4_656
Si4 Br1 Si1 70.36(2) 18_556 4_656
Si4 Br1 Si1 41.915(15) 15_655 4_656
Si1 Br1 Si1 109.5 . 4_656
Si1 Br1 Si1 70.5 13_666 4_656
Si1 Br1 Si1 180.0 16_565 4_656
P2 Br1 Si1 109.5 13_666 15_655
P2 Br1 Si1 70.5 . 15_655
P2 Br1 Si1 109.5 16_565 15_655
P2 Br1 Si1 70.5 4_656 15_655
P2 Br1 Si1 0.000(19) 15_655 15_655
P2 Br1 Si1 180.000(19) 3_566 15_655
P2 Br1 Si1 109.5 14_556 15_655
P2 Br1 Si1 70.5 2_665 15_655
Si4 Br1 Si1 138.085(15) 21_666 15_655
Si4 Br1 Si1 109.64(2) 17_666 15_655
Si4 Br1 Si1 70.36(2) 13_666 15_655
Si4 Br1 Si1 41.915(15) 9 15_655
Si4 Br1 Si1 109.64(2) . 15_655
Si4 Br1 Si1 70.36(2) 5 15_655
Si4 Br1 Si1 70.36(2) 10_656 15_655
Si4 Br1 Si1 41.915(15) 6_665 15_655
Si4 Br1 Si1 138.085(15) 3_566 15_655
Si4 Br1 Si1 109.64(2) 22_565 15_655
Si4 Br1 Si1 138.085(15) 18_556 15_655
Si4 Br1 Si1 41.915(15) 15_655 15_655
Si1 Br1 Si1 70.5 . 15_655
Si1 Br1 Si1 109.5 13_666 15_655
Si1 Br1 Si1 109.5 16_565 15_655
Si1 Br1 Si1 70.5 4_656 15_655
Te1 Br2A Te1 180.000(14) 21 9
Te1 Br2A Te1 65.807(4) 21 17
Te1 Br2A Te1 114.193(4) 9 17
Te1 Br2A Te1 65.807(4) 21 13
Te1 Br2A Te1 114.193(4) 9 13
Te1 Br2A Te1 65.807(4) 17 13
Te1 Br2A Te1 114.193(4) 21 5
Te1 Br2A Te1 65.807(4) 9 5
Te1 Br2A Te1 180.000(14) 17 5
Te1 Br2A Te1 114.193(4) 13 5
Te1 Br2A Te1 114.193(4) 21 .
Te1 Br2A Te1 65.807(4) 9 .
Te1 Br2A Te1 114.193(4) 17 .
Te1 Br2A Te1 180.000(14) 13 .
Te1 Br2A Te1 65.807(4) 5 .
Te1 Br2A Te1 124.952(14) 21 21_655
Te1 Br2A Te1 55.048(14) 9 21_655
Te1 Br2A Te1 65.807(4) 17 21_655
Te1 Br2A Te1 114.193(4) 13 21_655
Te1 Br2A Te1 114.193(4) 5 21_655
Te1 Br2A Te1 65.807(4) . 21_655
Te1 Br2A Te1 65.807(4) 21 13_556
Te1 Br2A Te1 114.193(4) 9 13_556
Te1 Br2A Te1 114.193(4) 17 13_556
Te1 Br2A Te1 124.952(14) 13 13_556
Te1 Br2A Te1 65.807(4) 5 13_556
Te1 Br2A Te1 55.048(14) . 13_556
Te1 Br2A Te1 114.193(4) 21_655 13_556
Te1 Br2A Te1 114.193(4) 21 17_565
Te1 Br2A Te1 65.807(4) 9 17_565
Te1 Br2A Te1 124.952(14) 17 17_565
Te1 Br2A Te1 65.807(4) 13 17_565
Te1 Br2A Te1 55.048(14) 5 17_565
Te1 Br2A Te1 114.193(4) . 17_565
Te1 Br2A Te1 114.193(4) 21_655 17_565
Te1 Br2A Te1 114.193(4) 13_556 17_565
Te1 Br2A Te1 55.048(14) 21 9_455
Te1 Br2A Te1 124.952(14) 9 9_455
Te1 Br2A Te1 114.193(4) 17 9_455
Te1 Br2A Te1 65.807(4) 13 9_455
Te1 Br2A Te1 65.807(4) 5 9_455
Te1 Br2A Te1 114.193(4) . 9_455
Te1 Br2A Te1 180.0 21_655 9_455
Te1 Br2A Te1 65.807(4) 13_556 9_455
Te1 Br2A Te1 65.807(4) 17_565 9_455
Te1 Br2A Te1 114.193(4) 21 1_554
Te1 Br2A Te1 65.807(4) 9 1_554
Te1 Br2A Te1 65.807(4) 17 1_554
Te1 Br2A Te1 55.048(14) 13 1_554
Te1 Br2A Te1 114.193(4) 5 1_554
Te1 Br2A Te1 124.952(14) . 1_554
Te1 Br2A Te1 65.807(4) 21_655 1_554
Te1 Br2A Te1 180.000(14) 13_556 1_554
Te1 Br2A Te1 65.807(4) 17_565 1_554
Te1 Br2A Te1 114.193(4) 9_455 1_554
Te1 Br2A Te1 65.807(4) 21 5_545
Te1 Br2A Te1 114.193(4) 9 5_545
Te1 Br2A Te1 55.048(14) 17 5_545
Te1 Br2A Te1 114.193(4) 13 5_545
Te1 Br2A Te1 124.952(14) 5 5_545
Te1 Br2A Te1 65.807(4) . 5_545
Te1 Br2A Te1 65.807(4) 21_655 5_545
Te1 Br2A Te1 65.807(4) 13_556 5_545
Te1 Br2A Te1 180.0 17_565 5_545
Te1 Br2A Te1 114.193(4) 9_455 5_545
Te1 Br2A Te1 114.193(4) 1_554 5_545
Te1 Te2B Te1 180.000(14) 21 9
Te1 Te2B Te1 65.807(4) 21 17
Te1 Te2B Te1 114.193(4) 9 17
Te1 Te2B Te1 65.807(4) 21 13
Te1 Te2B Te1 114.193(4) 9 13
Te1 Te2B Te1 65.807(4) 17 13
Te1 Te2B Te1 114.193(4) 21 5
Te1 Te2B Te1 65.807(4) 9 5
Te1 Te2B Te1 180.000(14) 17 5
Te1 Te2B Te1 114.193(4) 13 5
Te1 Te2B Te1 114.193(4) 21 .
Te1 Te2B Te1 65.807(4) 9 .
Te1 Te2B Te1 114.193(4) 17 .
Te1 Te2B Te1 180.000(14) 13 .
Te1 Te2B Te1 65.807(4) 5 .
Te1 Te2B Te1 124.952(14) 21 21_655
Te1 Te2B Te1 55.048(14) 9 21_655
Te1 Te2B Te1 65.807(4) 17 21_655
Te1 Te2B Te1 114.193(4) 13 21_655
Te1 Te2B Te1 114.193(4) 5 21_655
Te1 Te2B Te1 65.807(4) . 21_655
Te1 Te2B Te1 65.807(4) 21 13_556
Te1 Te2B Te1 114.193(4) 9 13_556
Te1 Te2B Te1 114.193(4) 17 13_556
Te1 Te2B Te1 124.952(14) 13 13_556
Te1 Te2B Te1 65.807(4) 5 13_556
Te1 Te2B Te1 55.048(14) . 13_556
Te1 Te2B Te1 114.193(4) 21_655 13_556
Te1 Te2B Te1 114.193(4) 21 17_565
Te1 Te2B Te1 65.807(4) 9 17_565
Te1 Te2B Te1 124.952(14) 17 17_565
Te1 Te2B Te1 65.807(4) 13 17_565
Te1 Te2B Te1 55.048(14) 5 17_565
Te1 Te2B Te1 114.193(4) . 17_565
Te1 Te2B Te1 114.193(4) 21_655 17_565
Te1 Te2B Te1 114.193(4) 13_556 17_565
Te1 Te2B Te1 55.048(14) 21 9_455
Te1 Te2B Te1 124.952(14) 9 9_455
Te1 Te2B Te1 114.193(4) 17 9_455
Te1 Te2B Te1 65.807(4) 13 9_455
Te1 Te2B Te1 65.807(4) 5 9_455
Te1 Te2B Te1 114.193(4) . 9_455
Te1 Te2B Te1 180.0 21_655 9_455
Te1 Te2B Te1 65.807(4) 13_556 9_455
Te1 Te2B Te1 65.807(4) 17_565 9_455
Te1 Te2B Te1 114.193(4) 21 1_554
Te1 Te2B Te1 65.807(4) 9 1_554
Te1 Te2B Te1 65.807(4) 17 1_554
Te1 Te2B Te1 55.048(14) 13 1_554
Te1 Te2B Te1 114.193(4) 5 1_554
Te1 Te2B Te1 124.952(14) . 1_554
Te1 Te2B Te1 65.807(4) 21_655 1_554
Te1 Te2B Te1 180.000(14) 13_556 1_554
Te1 Te2B Te1 65.807(4) 17_565 1_554
Te1 Te2B Te1 114.193(4) 9_455 1_554
Te1 Te2B Te1 65.807(4) 21 5_545
Te1 Te2B Te1 114.193(4) 9 5_545
Te1 Te2B Te1 55.048(14) 17 5_545
Te1 Te2B Te1 114.193(4) 13 5_545
Te1 Te2B Te1 124.952(14) 5 5_545
Te1 Te2B Te1 65.807(4) . 5_545
Te1 Te2B Te1 65.807(4) 21_655 5_545
Te1 Te2B Te1 65.807(4) 13_556 5_545
Te1 Te2B Te1 180.0 17_565 5_545
Te1 Te2B Te1 114.193(4) 9_455 5_545
Te1 Te2B Te1 114.193(4) 1_554 5_545
P2 Si1 P3 108.44(6) . .
P2 Si1 P3 108.44(6) . 9
P3 Si1 P3 110.49(6) . 9
P2 Si1 P3 108.44(6) . 5
P3 Si1 P3 110.49(6) . 5
P3 Si1 P3 110.49(6) 9 5
P2 Si1 Te1 71.34(3) . .
P3 Si1 Te1 64.32(4) . .
P3 Si1 Te1 75.09(4) 9 .
P3 Si1 Te1 173.84(4) 5 .
P2 Si1 Te1 71.34(3) . 9
P3 Si1 Te1 173.84(4) . 9
P3 Si1 Te1 64.32(4) 9 9
P3 Si1 Te1 75.09(4) 5 9
Te1 Si1 Te1 110.27(3) . 9
P2 Si1 Te1 71.34(3) . 5
P3 Si1 Te1 75.09(4) . 5
P3 Si1 Te1 173.84(4) 9 5
P3 Si1 Te1 64.32(4) 5 5
Te1 Si1 Te1 110.27(3) . 5
Te1 Si1 Te1 110.27(3) 9 5
P2 Si1 Br1 0.00(5) . .
P3 Si1 Br1 108.44(6) . .
P3 Si1 Br1 108.44(6) 9 .
P3 Si1 Br1 108.44(6) 5 .
Te1 Si1 Br1 71.34(3) . .
Te1 Si1 Br1 71.34(3) 9 .
Te1 Si1 Br1 71.34(3) 5 .
P2 Si1 Te1 108.36(2) . 17_565
P3 Si1 Te1 108.50(4) . 17_565
P3 Si1 Te1 112.52(5) 9 17_565
P3 Si1 Te1 2.29(4) 5 17_565
Te1 Si1 Te1 171.550(14) . 17_565
Te1 Si1 Te1 77.125(10) 9 17_565
Te1 Si1 Te1 62.358(17) 5 17_565
Br1 Si1 Te1 108.36(2) . 17_565
P2 Si1 Te1 108.36(2) . 13_556
P3 Si1 Te1 2.29(4) . 13_556
P3 Si1 Te1 108.50(4) 9 13_556
P3 Si1 Te1 112.52(5) 5 13_556
Te1 Si1 Te1 62.358(17) . 13_556
Te1 Si1 Te1 171.550(14) 9 13_556
Te1 Si1 Te1 77.125(10) 5 13_556
Br1 Si1 Te1 108.36(2) . 13_556
Te1 Si1 Te1 110.557(19) 17_565 13_556
P2 Si1 Te1 108.36(2) . 21_655
P3 Si1 Te1 112.52(5) . 21_655
P3 Si1 Te1 2.29(4) 9 21_655
P3 Si1 Te1 108.50(4) 5 21_655
Te1 Si1 Te1 77.125(10) . 21_655
Te1 Si1 Te1 62.358(17) 9 21_655
Te1 Si1 Te1 171.550(14) 5 21_655
Br1 Si1 Te1 108.36(2) . 21_655
Te1 Si1 Te1 110.557(19) 17_565 21_655
Te1 Si1 Te1 110.557(19) 13_556 21_655
P2 Si1 Te1 53.425(15) . 13_656
P3 Si1 Te1 109.19(4) . 13_656
P3 Si1 Te1 57.98(5) 9 13_656
P3 Si1 Te1 140.07(5) 5 13_656
Te1 Si1 Te1 44.88(2) . 13_656
Te1 Si1 Te1 65.52(2) 9 13_656
Te1 Si1 Te1 123.44(4) 5 13_656
Br1 Si1 Te1 53.425(15) . 13_656
Te1 Si1 Te1 141.878(16) 17_565 13_656
Te1 Si1 Te1 107.242(8) 13_556 13_656
Te1 Si1 Te1 58.671(6) 21_655 13_656
Si1 P2 Si4 107.89(6) . 9
Si1 P2 Si4 107.89(6) . 5
Si4 P2 Si4 111.00(6) 9 5
Si1 P2 Si4 107.89(6) . .
Si4 P2 Si4 111.00(6) 9 .
Si4 P2 Si4 111.00(6) 5 .
Si1 P2 Br1 180.00(12) . .
Si4 P2 Br1 72.11(6) 9 .
Si4 P2 Br1 72.11(6) 5 .
Si4 P2 Br1 72.11(6) . .
Si1 P2 Te1 72.79(3) . .
Si4 P2 Te1 60.89(4) 9 .
Si4 P2 Te1 170.99(4) 5 .
Si4 P2 Te1 76.79(4) . .
Br1 P2 Te1 107.21(3) . .
Si1 P2 Te1 72.79(3) . 5
Si4 P2 Te1 170.99(4) 9 5
Si4 P2 Te1 76.79(4) 5 5
Si4 P2 Te1 60.89(4) . 5
Br1 P2 Te1 107.21(3) . 5
Te1 P2 Te1 111.64(3) . 5
Si1 P2 Te1 72.79(3) . 9
Si4 P2 Te1 76.79(4) 9 9
Si4 P2 Te1 60.89(4) 5 9
Si4 P2 Te1 170.99(4) . 9
Br1 P2 Te1 107.21(3) . 9
Te1 P2 Te1 111.64(3) . 9
Te1 P2 Te1 111.64(3) 5 9
Si1 P2 Te1 107.375(19) . 13_656
Si4 P2 Te1 3.35(3) 9 13_656
Si4 P2 Te1 114.15(5) 5 13_656
Si4 P2 Te1 108.30(4) . 13_656
Br1 P2 Te1 72.625(19) . 13_656
Te1 P2 Te1 57.848(18) . 13_656
Te1 P2 Te1 167.689(14) 5 13_656
Te1 P2 Te1 79.642(10) 9 13_656
Si1 P2 Te1 107.375(19) . 21_665
Si4 P2 Te1 108.30(4) 9 21_665
Si4 P2 Te1 3.35(3) 5 21_665
Si4 P2 Te1 114.15(5) . 21_665
Br1 P2 Te1 72.625(19) . 21_665
Te1 P2 Te1 167.689(15) . 21_665
Te1 P2 Te1 79.642(10) 5 21_665
Te1 P2 Te1 57.848(18) 9 21_665
Te1 P2 Te1 111.483(18) 13_656 21_665
Si1 P2 Te1 107.375(19) . 17_566
Si4 P2 Te1 114.15(5) 9 17_566
Si4 P2 Te1 108.30(4) 5 17_566
Si4 P2 Te1 3.35(3) . 17_566
Br1 P2 Te1 72.625(19) . 17_566
Te1 P2 Te1 79.642(10) . 17_566
Te1 P2 Te1 57.848(18) 5 17_566
Te1 P2 Te1 167.689(14) 9 17_566
Te1 P2 Te1 111.483(18) 13_656 17_566
Te1 P2 Te1 111.483(18) 21_665 17_566
Si5 P3 Si1 106.20(7) . 15
Si5 P3 Si1 106.20(7) . .
Si1 P3 Si1 105.10(8) 15 .
Si5 P3 P3 124.31(7) . 2
Si1 P3 P3 106.79(5) 15 2
Si1 P3 P3 106.79(5) . 2
Si5 P3 Te1 74.54(5) . .
Si1 P3 Te1 176.16(6) 15 .
Si1 P3 Te1 78.13(3) . .
P3 P3 Te1 70.03(3) 2 .
Si5 P3 Te1 74.54(5) . 13_556
Si1 P3 Te1 78.13(3) 15 13_556
Si1 P3 Te1 176.16(6) . 13_556
P3 P3 Te1 70.03(3) 2 13_556
Te1 P3 Te1 98.57(5) . 13_556
Si5 P3 Te1 62.90(6) . 5
Si1 P3 Te1 69.28(5) 15 5
Si1 P3 Te1 69.28(5) . 5
P3 P3 Te1 172.79(3) 2 5
Te1 P3 Te1 114.12(4) . 5
Te1 P3 Te1 114.12(4) 13_556 5
Si5 P3 Te1 7.31(6) . 17_566
Si1 P3 Te1 102.00(6) 15 17_566
Si1 P3 Te1 102.00(6) . 17_566
P3 P3 Te1 131.629(18) 2 17_566
Te1 P3 Te1 79.13(3) . 17_566
Te1 P3 Te1 79.13(3) 13_556 17_566
Te1 P3 Te1 55.58(3) 5 17_566
Si5 P3 Te1 106.76(4) . 9_455
Si1 P3 Te1 3.80(2) 15 9_455
Si1 P3 Te1 108.33(5) . 9_455
P3 P3 Te1 103.688(18) 2 9_455
Te1 P3 Te1 172.36(4) . 9_455
Te1 P3 Te1 74.822(10) 13_556 9_455
Te1 P3 Te1 72.610(18) 5 9_455
Te1 P3 Te1 102.98(2) 17_566 9_455
Si5 P3 Te1 106.76(4) . 9
Si1 P3 Te1 108.33(5) 15 9
Si1 P3 Te1 3.80(2) . 9
P3 P3 Te1 103.688(18) 2 9
Te1 P3 Te1 74.822(10) . 9
Te1 P3 Te1 172.36(4) 13_556 9
Te1 P3 Te1 72.610(18) 5 9
Te1 P3 Te1 102.98(2) 17_566 9
Te1 P3 Te1 111.49(3) 9_455 9
Si5 P3 Te1 128.80(8) . 5_545
Si1 P3 Te1 104.25(5) 15 5_545
Si1 P3 Te1 104.25(5) . 5_545
P3 P3 Te1 4.483(18) 2 5_545
Te1 P3 Te1 72.72(3) . 5_545
Te1 P3 Te1 72.72(3) 13_556 5_545
Te1 P3 Te1 168.31(5) 5 5_545
Te1 P3 Te1 136.11(3) 17_566 5_545
Te1 P3 Te1 101.30(2) 9_455 5_545
Te1 P3 Te1 101.30(2) 9 5_545
Si5 P3 Br1 55.41(3) . .
Si1 P3 Br1 126.21(5) 15 .
Si1 P3 Br1 51.98(6) . .
P3 P3 Br1 125.557(12) 2 .
Te1 P3 Br1 57.399(17) . .
Te1 P3 Br1 127.82(4) 13_556 .
Te1 P3 Br1 57.284(16) 5 .
Te1 P3 Br1 52.890(13) 17_566 .
Te1 P3 Br1 129.70(3) 9_455 .
Te1 P3 Br1 51.871(8) 9 .
Te1 P3 Br1 127.044(14) 5_545 .
P2 Si4 P2 104.26(8) 14_556 .
P2 Si4 Si4 106.62(5) 14_556 3_566
P2 Si4 Si4 106.62(5) . 3_566
P2 Si4 Si5 106.11(8) 14_556 .
P2 Si4 Si5 106.11(8) . .
Si4 Si4 Si5 125.37(7) 3_566 .
P2 Si4 Te1 174.29(6) 14_556 5
P2 Si4 Te1 80.86(3) . 5
Si4 Si4 Te1 69.10(3) 3_566 5
Si5 Si4 Te1 74.45(5) . 5
P2 Si4 Te1 80.86(3) 14_556 17_566
P2 Si4 Te1 174.29(6) . 17_566
Si4 Si4 Te1 69.10(3) 3_566 17_566
Si5 Si4 Te1 74.45(5) . 17_566
Te1 Si4 Te1 93.91(5) 5 17_566
P2 Si4 Br1 65.98(6) 14_556 .
P2 Si4 Br1 65.98(6) . .
Si4 Si4 Br1 69.30(3) 3_566 .
Si5 Si4 Br1 165.33(9) . .
Te1 Si4 Br1 114.73(4) 5 .
Te1 Si4 Br1 114.73(4) 17_566 .
P2 Si4 Te1 67.74(5) 14_556 .
P2 Si4 Te1 67.74(5) . .
Si4 Si4 Te1 169.66(3) 3_566 .
Si5 Si4 Te1 64.97(6) . .
Te1 Si4 Te1 117.09(4) 5 .
Te1 Si4 Te1 117.09(4) 17_566 .
Br1 Si4 Te1 100.36(4) . .
P2 Si4 Te1 103.24(7) 14_556 13_556
P2 Si4 Te1 103.24(7) . 13_556
Si4 Si4 Te1 130.335(16) 3_566 13_556
Si5 Si4 Te1 4.97(6) . 13_556
Te1 Si4 Te1 77.72(3) 5 13_556
Te1 Si4 Te1 77.72(3) 17_566 13_556
Br1 Si4 Te1 160.36(4) . 13_556
Te1 Si4 Te1 60.00(3) . 13_556
P2 Si4 Te1 5.54(2) 14_556 9_556
P2 Si4 Te1 108.61(5) . 9_556
Si4 Si4 Te1 101.777(17) 3_566 9_556
Si5 Si4 Te1 107.57(4) . 9_556
Te1 Si4 Te1 168.80(4) 5 9_556
Te1 Si4 Te1 76.356(10) 17_566 9_556
Br1 Si4 Te1 65.816(18) . 9_556
Te1 Si4 Te1 72.950(18) . 9_556
Te1 Si4 Te1 105.10(2) 13_556 9_556
P2 Si4 Te1 108.61(5) 14_556 9
P2 Si4 Te1 5.54(2) . 9
Si4 Si4 Te1 101.777(17) 3_566 9
Si5 Si4 Te1 107.57(4) . 9
Te1 Si4 Te1 76.356(10) 5 9
Te1 Si4 Te1 168.80(4) 17_566 9
Br1 Si4 Te1 65.816(18) . 9
Te1 Si4 Te1 72.950(18) . 9
Te1 Si4 Te1 105.10(2) 13_556 9
Te1 Si4 Te1 112.72(3) 9_556 9
P2 Si4 Te1 102.89(5) 14_556 1_565
P2 Si4 Te1 102.89(5) . 1_565
Si4 Si4 Te1 6.463(18) 3_566 1_565
Si5 Si4 Te1 131.83(8) . 1_565
Te1 Si4 Te1 73.21(3) 5 1_565
Te1 Si4 Te1 73.21(3) 17_566 1_565
Br1 Si4 Te1 62.84(3) . 1_565
Te1 Si4 Te1 163.20(5) . 1_565
Te1 Si4 Te1 136.80(3) 13_556 1_565
Te1 Si4 Te1 98.33(2) 9_556 1_565
Te1 Si4 Te1 98.33(2) 9 1_565
P3 Si5 P3 111.37(14) . 14_556
P3 Si5 Si4 109.04(3) . .
P3 Si5 Si4 109.04(3) 14_556 .
P3 Si5 Si4 109.04(3) . 15
P3 Si5 Si4 109.04(3) 14_556 15
Si4 Si5 Si4 109.27(13) . 15
P3 Si5 Te1 167.83(10) . 17_566
P3 Si5 Te1 80.80(5) 14_556 17_566
Si4 Si5 Te1 65.18(6) . 17_566
Si4 Si5 Te1 65.18(6) 15 17_566
P3 Si5 Te1 80.80(5) . 5
P3 Si5 Te1 167.83(10) 14_556 5
Si4 Si5 Te1 65.18(6) . 5
Si4 Si5 Te1 65.18(6) 15 5
Te1 Si5 Te1 87.03(7) 17_566 5
P3 Si5 Te1 67.14(5) . 13_556
P3 Si5 Te1 67.14(5) 14_556 13_556
Si4 Si5 Te1 171.80(10) . 13_556
Si4 Si5 Te1 78.93(5) 15 13_556
Te1 Si5 Te1 119.985(2) 17_566 13_556
Te1 Si5 Te1 119.985(2) 5 13_556
P3 Si5 Te1 67.14(5) . .
P3 Si5 Te1 67.14(5) 14_556 .
Si4 Si5 Te1 78.93(5) . .
Si4 Si5 Te1 171.80(10) 15 .
Te1 Si5 Te1 119.985(2) 17_566 .
Te1 Si5 Te1 119.985(2) 5 .
Te1 Si5 Te1 92.87(7) 13_556 .
P3 Si5 Br1 104.708(18) . .
P3 Si5 Br1 104.708(18) 14_556 .
Si4 Si5 Br1 8.60(5) . .
Si4 Si5 Br1 117.87(9) 15 .
Te1 Si5 Br1 70.94(3) 17_566 .
Te1 Si5 Br1 70.94(3) 5 .
Te1 Si5 Br1 163.20(6) 13_556 .
Te1 Si5 Br1 70.329(12) . .
P3 Si5 Br1 104.708(18) . 1_455
P3 Si5 Br1 104.708(18) 14_556 1_455
Si4 Si5 Br1 117.87(9) . 1_455
Si4 Si5 Br1 8.60(5) 15 1_455
Te1 Si5 Br1 70.94(3) 17_566 1_455
Te1 Si5 Br1 70.94(3) 5 1_455
Te1 Si5 Br1 70.329(12) 13_556 1_455
Te1 Si5 Br1 163.20(6) . 1_455
Br1 Si5 Br1 126.47(5) . 1_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Te1 Si4 3.2719(13) 10_656
Te1 Si4 3.2719(13) 9
Te1 Si4 3.2719(13) 21_656
Te1 Si4 3.2719(13) 22
Te1 P3 3.4329(13) 2
Te1 P3 3.4329(13) 13_556
Te1 P3 3.4329(13) .
Te1 P3 3.4329(13) 14_556
Te1 Si5 3.4729(18) 21_656
Te1 Si5 3.4729(18) 9
Te1 Si5 3.5908(17) 13_556
Te1 Si5 3.5908(17) .
Te1 P2 3.6972(6) 14_556
Te1 P2 3.6972(6) 16
Te1 P2 3.6972(6) .
Te1 P2 3.6972(6) 3_556
Te1 Si1 3.7277(7) 16
Te1 Si1 3.7277(7) 14_556
Te1 Si1 3.7277(7) .
Te1 Si1 3.7277(7) 3_556
Te1 P3 3.8512(17) 9
Te1 P3 3.8512(17) 23_556
Te1 Si4 3.8892(17) 3_556
Te1 Si4 3.8892(17) .
Te1 Te1 4.7824(15) 13_656
Br1 P2 3.170(2) 13_666
Br1 P2 3.170(2) .
Br1 P2 3.170(2) 16_565
Br1 P2 3.170(2) 4_656
Br1 P2 3.170(2) 15_655
Br1 P2 3.170(2) 3_566
Br1 P2 3.170(2) 14_556
Br1 P2 3.170(2) 2_665
Br1 Si4 3.3022(17) 21_666
Br1 Si4 3.3022(17) 17_666
Br1 Si4 3.3022(17) 13_666
Br1 Si4 3.3022(17) 9
Br1 Si4 3.3022(17) .
Br1 Si4 3.3022(17) 5
Br1 Si4 3.3022(17) 10_656
Br1 Si4 3.3022(17) 6_665
Br1 Si4 3.3022(17) 3_566
Br1 Si4 3.3022(17) 22_565
Br1 Si4 3.3022(17) 18_556
Br1 Si4 3.3022(17) 15_655
Br1 Si1 5.456(2) .
Br1 Si1 5.456(2) 13_666
Br1 Si1 5.456(2) 16_565
Br1 Si1 5.456(2) 4_656
Br1 Si1 5.456(2) 15_655
Br2A Te1 5.6304(4) 21
Br2A Te1 5.6304(4) 9
Br2A Te1 5.6304(4) 17
Br2A Te1 5.6304(4) 13
Br2A Te1 5.6304(4) 5
Br2A Te1 5.6304(4) 21_655
Br2A Te1 5.6304(4) 13_556
Br2A Te1 5.6304(4) 17_565
Br2A Te1 5.6304(4) 9_455
Br2A Te1 5.6304(4) 1_554
Br2A Te1 5.6304(4) 5_545
Te2B Te1 5.6304(4) 21
Te2B Te1 5.6304(4) 9
Te2B Te1 5.6304(4) 17
Te2B Te1 5.6304(4) 13
Te2B Te1 5.6304(4) 5
Te2B Te1 5.6304(4) 21_655
Te2B Te1 5.6304(4) 13_556
Te2B Te1 5.6304(4) 17_565
Te2B Te1 5.6304(4) 9_455
Te2B Te1 5.6304(4) 1_554
Te2B Te1 5.6304(4) 5_545
Si1 P2 2.286(3) .
Si1 P3 2.3216(13) .
Si1 P3 2.3216(13) 9
Si1 P3 2.3216(13) 5
Si1 Te1 3.7277(7) 9
Si1 Te1 3.7277(7) 5
Si1 Te1 5.7514(9) 17_565
Si1 Te1 5.7514(9) 13_556
Si1 Te1 5.7514(9) 21_655
Si1 Te1 6.6351(14) 13_656
P2 Si4 2.3181(12) 9
P2 Si4 2.3181(12) 5
P2 Si4 2.3181(12) .
P2 Te1 3.6972(6) 5
P2 Te1 3.6972(6) 9
P2 Te1 5.5832(8) 13_656
P2 Te1 5.5832(8) 21_665
P2 Te1 5.5832(8) 17_566
P3 Si5 2.310(2) .
P3 Si1 2.3216(13) 15
P3 P3 2.345(3) 2
P3 Te1 3.4329(13) 13_556
P3 Te1 3.8512(17) 5
P3 Te1 5.7515(18) 17_566
P3 Te1 6.0410(10) 9_455
P3 Te1 6.0410(10) 9
P3 Te1 6.1845(17) 5_545
Si4 P2 2.3181(12) 14_556
Si4 Si4 2.334(3) 3_566
Si4 Si5 2.335(2) .
Si4 Te1 3.2719(13) 5
Si4 Te1 3.2719(13) 17_566
Si4 Te1 5.9113(18) 13_556
Si4 Te1 5.9977(9) 9_556
Si4 Te1 5.9977(9) 9
Si4 Te1 6.1996(17) 1_565
Si5 P3 2.310(2) 14_556
Si5 Si4 2.335(2) 15
Si5 Te1 3.4729(18) 17_566
Si5 Te1 3.4729(18) 5
Si5 Te1 3.5908(17) 13_556
Si5 Br1 5.5924(12) 1_455
